Impact of Competitive Processes on Controlled Radical Polymerization Nicholas Ballard,† Simone Rusconi,‡ Elena Akhmatskaya,‡,§ Dmitri Sokolovski,§,∥ José C. de la Cal,† and José M. Asua*,† †
POLYMAT and Grupo de Ingeniería Química, Dpto. de Química Aplicada, University of the Basque Country UPV/EHU, Joxe Mari Korta Zentroa, Tolosa Etorbidea 72, 20018 Donostia/San Sebastián, Spain ‡ Basque Center for Applied Mathematics (BCAM), Alameda de Mazarredo 14, 48009 Bilbao, Spain § Ikerbasque, Basque Foundation for Science, 48011 Bilbao, Spain ∥ Department of Physical Chemistry, University of the Basque Country UPV/EHU, 48940 Leioa, Spain S Supporting Information *
ABSTRACT: The kinetics of radical polymerization have been systematically studied for nearly a century and in general are well understood. However, in light of recent developments in controlled radical polymerization many kinetic anomalies have arisen. These unexpected results have been largely considered separate, and various, as yet inconclusive, debates as to the cause of these anomalies are ongoing. Herein we present a new theory on the cause of changes in kinetics under controlled radical polymerization conditions. We show that where the fast, intermittent deactivation of radical species takes place, changes in the relative rates of the competitive reactions that exist in radical polymerization can occur. To highlight the applicability of the model, we demonstrate that the model explains well the reduction in branching in acrylic polymers in RAFT polymerization. We further show that such a theory may explain various phenomena in controlled radical polymerization and may be exploited to design precise macromolecular architectures.
polymer.1−12 Transfer to polymer in acrylic monomers has been shown to be mainly due to intramolecular transfer via a six-membered ring transition state, resulting in a midchain radical.13−17 In general, for most polymerizations which are conducted at a temperature of ti
pi (t ) = kit
⎛ t − ti ⎞ pi (t ) = kiti exp⎜ − ⎟ τi ⎠ ⎝
Pi(t < ti) =
Pi(t > ti) =
kit ′ dt ′ = ti
kit ′ dt ′+
kit 2 2
⎛ t ′ − ti ⎞ kiti exp⎜ − ⎟ dt ′ τi ⎠ ⎝
⎛ ⎛ t − ti ⎞⎞ kt = i i + kitiτi⎜⎜1 − exp⎜ − ⎟⎟⎟ 2 τi ⎠⎠ ⎝ ⎝ 2
As t → ∞, then Pi(∞) = 1; thus, the slope of the initial part of the curve is given by 2 2tiτi + ti 2
and the probability distribution can be rewritten as 0 < t < ti
t > ti
pi (t ) =
pi (t ) =
2t 2tiτi + ti 2
⎛ t − ti ⎞ exp⎜ − ⎟ τi ⎠ 2tiτi + ti ⎝
This curve describes the probability distribution with the area beneath it being 1 and with a mean, being equal to the characteristic time scale for a reaction to occur. t i̅ =
tpi (t ) dt =
⎛t3 ⎛ ti ⎞⎞ 2 i 2 ⎜ + + τ t 1 ⎜ ⎟⎟⎟ ⎜ i i τi ⎠⎠ 2tiτi + ti 2 ⎝ 3 ⎝ (12)
The intrinsic rate constant for a given reaction is given by 1/ ti̅ , which for propagation of secondary radicals is kp,int[M] and for backbiting kbb,int and for deactivation of a propagating secondary radical by RAFT agent, kadd,int[RAFT]. It is worth discussing the eﬀect of the present theory on the relationship between the intrinsic rate coeﬃcient and the rate coeﬃcient determined from experimental measurements. When the kinetic rate coeﬃcient of a given reaction is determined independently, without the inﬂuence of other processes, both the intrinsic and experimentally measured rate coeﬃcients coincide. This is the case for the propagation rate coeﬃcient for secondary radicals as measured by PLP (kp = kp,int). However, when, as in the case of backbiting, the rate coeﬃcient is determined in the presence of other processes (i.e., propagation), then the relationship between the intrinsic and experimentally determined rate coeﬃcient is not straightforward. This would also cause issues with the calculation of any kinetic rate constant in the presence of competitive reactions. The experimental data used in this work (RAFT polymerization of n-butyl acrylate) showed that the reactions were not carried out under isothermal conditions. Therefore, the values of the rate coeﬃcients kp and kbb are unknown, and it was decided to normalize the coeﬃcients by “kp[M]*”,where [M]* = 1 mol L−1. The normalization allows for relative probabilities to be calculated without taking into account changes in temperature throughout the polymerization and leads to a similar set of equations:
where the parameter ki determines the gradient of the initial part of probability density function up to point in time ti and the parameter τi is similar to the rate constant in classical radical kinetics, describing the decay of the exponential function in the probability density function after time ti. The probability of a reaction having occurred by time t, P(t), is therefore given by
for 0 < t * < ti*: E
pi (t *) =
2t * 2 * ti + 2ti*τi*
dx.doi.org/10.1021/ma501267a | Macromolecules XXXX, XXX, XXX−XXX
Scheme 2. Reactions Scheme Used for Monte Carlo Kinetic Model
Table 1. Details of RAFT Reactions temp (°C) 80
[M] (mol L−1)
[initiator] (mM) 10
DTTC DTTC CPTP MPCP 110
7.25 DTTC DTTC MPCP MPCP
0 5.0 100 9.9 12.1 0 4.5 33 5.4 28
0.80 0.81 0.69 0.72 0.70 0.82 0.80 0.80 0.82 0.80
f Brb 1.82 1.71 1.34 1.55 2.03 2.85 2.39 1.55 3.09 2.89
± ± ± ± ± ± ± ± ± ±
0.02 0.14 0.19 0.08 0.16 0.16 0.12 0.08 0.12 0.16
RAFT agents used were 2-(dodecylthiocarbonothioylthio)-2-methylpropionic acid (DTTC), methyl 2-[methyl(4-pyridinyl)carbamothioylthio]propionate (MPCP), and 4-cyano-4-(phenylcarbonothioylthio)pentanoic acid (CPTP). bError in branching fraction is calculated from the inverse of the signal-to-noise ratio of the quaternary carbon peak (see Methods section).
for t ∗ > ti*:
pi (t *) =
⎛ t* − t* ⎞ i ⎜− ⎟ exp 2 * * * * τi ti + 2ti τi ⎝ ⎠
of 10 s. Apodization was achieved using an exponential window function equivalent to a line width of 10 Hz. 1D 13C DEPT-135 spectra were acquired for 16 000 transients using single pulse excitation, using a 5.5 μs 90° pulse, inverse gated waltz16 decoupling to avoid NOE eﬀects, and a relaxation delay of 10 s. Apodization was achieved using an exponential window function equivalent to a line width of 3 Hz. 2D NMR spectra were recorded in HSQC and HMBC experiments. The spectral widths for the HSQC experiment were 5000 and 25 000 Hz for the 1H and the 13C dimensions, respectively. The number of collected complex points was 2048 for the 1H dimension with a recycle delay of 5 s. The number of transients was 64, and 256 time increments were recorded in the 13C dimension. The 1JCH used was 140 Hz. The J-coupling evolution delay was set to 3.2 ms. The squared cosine-bell apodization function was applied in both dimensions. Prior to Fourier transformation, the data matrices were zero ﬁlled to 1024 points in the 13C dimension. The branching fraction, f Br, of the polymers was calculated from quantitative 13C spectra from the ratio of the integral of the quaternary carbon peak (45−49 ppm) and the methyl group of the butyl ester (11−14 pm).9 The methyl group of the butyl ester was used instead of the tertiary carbon in the backbone for comparison as reported in the cited article due to the superior resolution of this peak and overlap of some peaks from the RAFT agents used with the backbone carbon signals in 13C NMR. The error in the branching fraction was calculated from the inverse of the signal-to-noise ratio of the quaternary carbon peak. This approach is valid where the integral area of the quaternary peak is substantially smaller than the peak against which it is compared. RAFT Polymerization. RAFT polymerizations were conducted in two-neck round-bottomed ﬂasks with a ﬁtted reﬂux condenser under an atmosphere of nitrogen. In a typical reaction, the RAFT agent, monomer, solvent, and initiator were mixed to dissolution, and then the solution was bubbled with nitrogen for 20 min. The bulk reactions were conducted on a 2 g scale while the solution polymerizations were conducted on a 5 g scale. The reaction was heated to reaction temperature and left for 3 h (bulk polymerizations at 80 °C) or 1 h
where t* = t × kp[M]*; ti* = ti × kp[M]*, and τi* = τi × kp[M]*. Then the mean values of the normalized distributions are kp[M]*/kp[M] = 1/[M] for propagation, kp[M]*/kbb,int for backbiting, and kp[M]*/kadd,int[RAFT] for the addition of secondary radicals to the RAFT. Note that for propagation and deactivation, t*i and τ*i are divided by [M] and [RAFT] for diﬀerent conversions or diﬀerent experiments. The summary of the competing reactions considered in the kinetic model is shown in Scheme 2.
Materials. n-Butyl acrylate (Quimidroga, technical grade) was puriﬁed by distillation and was kept at −20 °C until use. The initiators azobis(isobutyronitrile) (AIBN, Aldrich, 98%) and 1,1′-azobis(cyclohexanecarbonitrile) (ACHN, Aldrich, 97%) and the RAFT agents 2-(dodecylthiocarbonothioylthio)-2-methylpropionic acid (DTTC, Strem, 97%), methyl 2-propionate methyl(4-pyridinyl)carbamodithioate (MPCP, Aldrich, 97%), and 4-cyano-4(phenylcarbonothioylthio)pentanoic acid (CPTP, Aldrich, 97%) were used as received. All other solvents were purchased from Scharlab and were used without puriﬁcation. Methods. NMR spectra were recorded at 25 °C in CDCl3 at a concentration of 200 mg mL−1 on a Bruker AVANCE 500 MHz equipped with a z-gradient double resonance probe. 1D 1H spectra were acquired by use of 32K data points which were zero-ﬁlled to 64K data points prior to Fourier transformation. 1D 13C spectra were recorded at a 13C Larmor frequency of 125.77 MHz. The spectra were recorded using 20 000 transients. Quantitative 13C spectra were recorded using single pulse excitation, using a 5.5 μs 90° pulse, inverse gated waltz16 decoupling to avoid NOE eﬀects, and a relaxation delay F
dx.doi.org/10.1021/ma501267a | Macromolecules XXXX, XXX, XXX−XXX
(solution polymerization 110 °C). The fractional conversion, X, was calculated gravimetrically. The reactions performed are detailed in Table 1.
Table 2. Results of Polymerization of n-Butyl Acrylate and Corresponding Fit of Model Data Based on Parameter Estimation Approach
RESULTS The proposed model was veriﬁed experimentally by using RAFT polymerization with varying concentrations of RAFT agent to observe the diﬀerence in the branching fraction, f Br, which is in turn dependent on the rate of transfer to polymer. Table 1 shows that for the trithiocarbonate RAFT agent, DTTC, in both solution and bulk polymerizations the branching fraction decreases with increasing DTTC concentration. This result is in qualitative agreement with the predictions of the linear−exponential model that states that if the deactivation time (which for a RAFT polymerization decreases as kadd,int[RAFT] increases) decreases, then the rate of transfer to polymer relative to propagation will be reduced and therefore the branching fraction should decrease (see Figure 2b). This eﬀect is also observable using the more active dithiobenzoate RAFT agent, CPTP, for which the branching is reduced substantially even at low concentrations. Therefore, by changing the RAFT agent, and thus the value of rate constant kadd,int, or its concentration, the branching fraction can be reduced relative to that of radical polymerization. Similar eﬀects have previously been observed in nitroxide-mediated polymerizations by using excess of free nitroxide resulting in a lower branching fraction.30 We also performed experiments with a dithiocarbamate RAFT agent (MPCP) which typically gives very poor control of acrylate polymerizations because of the low chain transfer constant. When MPCP was used, no change in the branching fraction compared to the conventional radical polymerizations was observed. In terms of the linear− exponential model, this is explained by the fact that the low kadd,int results in a long deactivation time that is of the same order of magnitude or greater than the characteristic time for backbiting, and hence it will not aﬀect the rate of backbiting. Following these experimental observations, we explored the possibility of quantitative ﬁtting of the data to the proposed model. In order to implement this, we performed a series of Monte Carlo simulations, and the unknown parameters were estimated using a Nelder−Mead simplex algorithm for the data obtained with the trithiocarbonate RAFT agent, DTTC (see Supporting Information for the description of the algorithm). We assumed all reactions to be described by the linear− exponential density functions such that the unknown parameters were ti* (i = 1, 2, 3 for propagation, backbiting, and radical addition to RAFT agent; see Scheme 2), kbb,int/ kp[M]*, and kadd,int[RAFT]*/kp[M]*, where [RAFT]* = 1 mol L−1 and [M]* = 1 mol L−1. The results of the model ﬁt to the bulk and solution polymerization data are given in Table 2. The model provides a good description for the data in every case and predicts the trend of decreasing branching fraction with increasing RAFT agent concentration. Moreover, this result is universal in explaining the decrease in branching density in all controlled radical polymerizations in which the deactivation time is typically much faster than the characteristic time for backbiting. The good agreement between the model and the experimental data can be seen in Figure 4. The linear− exponential distribution model would also explain why in both pulsed laser polymerizations and chain transfer agent mediated polymerizations branching is reduced since both introduce a competitive event that is signiﬁcantly faster than the character-
RAFT concn (mol L−1)
monomer concn (mol L−1)
0.0 5 × 10−3 100 × 10−3 0.0 4.5 × 10−3 33 × 10−3
6.9 6.9 6.9 2.25 2.25 2.25
exptl branching fraction (%)
model prediction branching fraction (%)
± ± ± ± ± ±
1.78a 1.73a 1.33a 2.81b 2.44b 1.54b
1.82 1.71 1.34 2.85 2.39 1.55
0.02 0.14 0.19 0.16 0.12 0.08
Estimated values of the parameters t1* = 6.89 × 10−2, t2* = 8.39 × 10−2, t3* = 5.48 × 10−3, kbb,int/kp[M]* = 7.33 × 10−2, and kadd,int[RAFT]*/kp[M]* = 23.1. bEstimated values of the parameters t1* =7.97 × 10−2, t2* =1.28, t3* =3.85 × 10−4, kbb,int/kp[M]* = 6.18 × 10−2, and kadd,int[RAFT]*/kp[M]* = 49.6. a
Figure 4. Agreement between model (open symbols) and experimental data (ﬁlled symbols) for branching fraction in RAFT polymerization of n-butyl acrylate at 80 °C in bulk (squares) and 110 °C in solution (circles) according to recipes in Table 1.
istic time for backbiting and will reduce its rate relative to that of propagation. The shape of the probability density functions can evolve with conversion due to changes in the concentrations of the chemical species involved. Figure 5 shows the normalized probability density distribution for propagation, chain transfer to RAFT agent, and backbiting at low and high conversion for a RAFT solution polymerization conducted at [M0] = 2.25 mol L−1 and [RAFT] = 33 mmol L−1. It can be observed that at low conversion the probability density distributions for chain transfer to RAFT agent and propagation are similar, as expected due to a similar relative rate, while the probability density distribution for backbiting both has a relatively larger linear region (indicating this process is signiﬁcantly less likely to occur at short times) and has a slower exponential decay (indicating a slower average rate of reaction). At high conversion, the probability density functions for chain transfer to RAFT agent and backbiting are unchanged, since the RAFT agent concentration is constant and backbiting is concentration independent, whereas the probability density function for propagation is changed signiﬁcantly and exhibits a slightly longer linear region and signiﬁcantly slower decay. Although the parameter estimation process gives a good ﬁt to the data, it must be highlighted that it is an ill-posed estimation; namely, it presents more than one solution as shown in the Supporting Information. Therefore, at this stage it is diﬃcult to assign these values with conﬁdence. One of the main diﬃculties G
dx.doi.org/10.1021/ma501267a | Macromolecules XXXX, XXX, XXX−XXX
Figure 5. Changing of probability density functions from low conversion (0%, left) to high conversion (80%, right) for RAFT solution polymerization using [M] = 2.25 M, [RAFT] = 33 mM, and parameters from results in Table 2. Propagation (squares), addition of radical to RAFT agent (triangles), and backbiting (circles). Inset shows the distributions at short times. The normalized time is given by t* = t × kp[M]* where [M]* = 1.
imposition of controlled polymerization conditions signiﬁcantly diminishes the extent of transfer in this case.48 Extending further it has been shown that, in general, copper(0)-mediated polymerization has excellent end-group ﬁdelity in comparison to other atom transfer processes.49−52 Again, the current model would predict that under conditions of fast deactivation, such is the case in these polymerizations, termination and transfer events, which are typically long time scale, should be reduced with respect to propagation, thus allowing for the ultrahighmolecular-weight polymers with near to 0 mol % termination that have been seen already. Although for acrylates this may be explained simply by the large kp/kt ratio, for vinyl chloride it has been shown that the molecular weight can exceed that of free radical polymerization45 which can only be the case when molecular weight limiting reactions such as chain transfer to monomer and termination are reduced in comparison to propagation. Extending even further, it may be considered that even short time events such as propagation may be reduced when the deactivation time is on a similar time scale to that of propagation. In the simulations conducted herein we were mainly concerned with the relative rate of propagation to backbiting that results in a reduction in branching fraction when RAFT agents were used, but the rates of polymerization were also calculated. Retardation phenomena have been reported in RAFT polymerizations when certain RAFT agents are used, particularly the highly active dithiobenzoates, and the cause of this is the subject of an unresolved debate in the literature.53,54 Figure 6 shows the results from the Monte Carlo simulations that predict the change in the polymerization rate for varying concentrations of RAFT agent relative to the rate of polymerization for a conventional radical polymerization using the parameters estimated for the solution polymerization experiments. The results have been calculated for solution polymerization, assuming instantaneous fragmentation of the RAFT intermediate and represent the average propagation rate between 0 and 0.82 conversion according to
is that the physical origin of the time scale in which the linear part of the probability distribution function exists is not yet clear. For the eﬀect to be of signiﬁcance, the linear region time scale must be at least remotely similar to that of the average transient radical lifetime. In this case, limitations at short times due to diﬀusion or molecular rearrangement seem unlikely, but alternative possibilities may be explored. For example, the addition of hydroxyl radicals to alkenes has been shown to proceed via a two-step process involving long-range transition states41−43 which would not be isolatable and would not change the average rate of reaction but would result in a hypoexponential type of probability density function as described herein. Although the examples used in this paper focus on intramolecular chain transfer to polymer in acrylate polymerizations, it is important to note that the same concept should be applicable to all kinetic events that occur in radical processes and in a broader sense to all chemical reactions. Indeed, even after a brief foray into the literature on the subject of controlled radical polymerization, one will encounter numerous examples of a seemingly unexplainable reduction in reactivity or enhanced selectivity when deactivation rates are high. Table 3 summarizes these examples including the theories currently oﬀered to explain them. This table also shows that all these ﬁndings can be explained by means of the model based on a hypoexponential probability density distribution. It is very diﬃcult to say at this stage to what extent the current theories are incorrect (if at all), whether the proposed theory is the cause for the change in reactivity or whether the change in reactivity is due to multiple causes acting in tandem. In order to make ﬁrm statements further, experimental work must come to light that is capable of discerning between these mechanisms which will be a decidedly tricky task. In the single electron transfer−degenerative chain transfer living radical polymerization (SET-DTLRP) of vinyl chloride, for example, it has been shown that defect-free samples can be prepared.44−47 In light of the theory proposed here it may be as a result of the reduced transient radical lifetime that defects, which for vinyl chloride polymerization are largely caused by transfer to polymer, are reduced. In addition, similar polymerizations conducted in aqueous media suggested that chain transfer to the poly(vinyl alcohol) stabilizer employed does not occur.47,48 Given that chain transfer to PVA in conventional radical polymerization of PVC is extensive and leads to a characteristic skin of the resulting particles, it is clear that the
relative average propagation rate =
k p[M] (k p[M])[RAFT] = 0
The rate of polymerization was calculated taking into account the complete kinetic scheme including backbiting and propagation from the tertiary radical but does not include H
dx.doi.org/10.1021/ma501267a | Macromolecules XXXX, XXX, XXX−XXX
high deactivation rate suppresses termination and chain transfer processes
Figure 6. Predicted change in relative rate of polymerization compared to conventional radical polymerization with increasing RAFT agent concentration for solution polymerization ([M] = 2.25 M and using parameters given in Table 2).
low termination rates due to (i) low copper concentrations60 and (ii) low termination rate coeﬃcients relative to propagation of monomers employed61,62
eﬀects due to slow fragmentation of the RAFT agent or termination of RAFT adduct radicals. It can clearly be observed that, in keeping with experimental observations, the theory qualitatively predicts that the relative rate of propagation is reduced compared to the free radical case. Such a prediction would mean a reevaluation of the fundamental principle on which the kinetics of controlled radical polymerization are built, in that it would appear that while rate coeﬃcients calculated from conventional radical polymerizations may be applicable in some instances, the short lifetime of the transient radical may cause signiﬁcant diﬀerences in relative rates. The application of this single concept conveniently explains a number of ongoing debates and unexplained phenomena in the ﬁeld of radical polymerization as summarized in Table 3. In light of the propsed model, it would appear that polymerization under conditions of high deactivation rates may allow for polymerizations of increased speciﬁcity with decreased termination and decreased chain transfer events, thus allowing for synthesis of polymers with precise, predetermined microstructure.
CONCLUSION In conclusion, we have presented a new model for the relative reactivity in the presence of competitive processes that shows that under conditions of rapid radical deactivation long scale processes such as transfer to polymer can be suppressed. This model is particularly useful for explaining the enhanced selectivity of radicals in the presence of a reversible deactivation process in radical polymerization. We have shown that, based on the use of a hypoexponential-like probability density function, good agreement between the model and experimental data for branching in RAFT polymerization of acrylic monomers is given. In addition, we have highlighted the possibility for the application of the model to various other kinetic processes in radical polymerizations. Thus, using a single concept, a broad range of unresolved debates can be explained. It is important to note that the model presented should be generally applicable to all chemical reactions. Application of the knowledge provided by such a model should allow for the development of highly selective radical polymerization processes potentially avoiding all chain transfer and termination events.
branching reduced when high concentrations of chain transfer agent used in radical polymerization31,32 pulsed laser polymerization of acrylates at high frequency gives accurate kp values at high temperatures34 reduction in rate of polymerization in RAFT-mediated polymerizations53,54 defect-free poly(vinyl chloride) formed by SETDTLRP45 absence of chain transfer to PVA in SET-DTLRP of PVC in aqueous media48 high chain-end ﬁdelity/near-zero termination in copper(0)-mediated radical polymerizations49,52,59 ultrahigh-Mw polymers possible with copper(0)-mediated radical polymerizations/SET-DTLRP45,50
linear−exponential probability distribution explanation
intermittent deactivation of transient radical results in decrease in rate of backbiting relative to propagation reduction in radical lifetime due to chain transfer to CTA results in decrease in backbiting rate reduction in radical lifetime due to chain termination induced by fast laser pulse results in decrease in backbiting rate either (i) termination/side reactions of intermediate RAFT adduct55−57 or (ii) slow high deactivation rate for certain RAFT agents reduces the transient radical fragmentation of intermediate RAFT adduct58 lifetime so td̅ eactivation ≈ tp̅ ropagation reducing propagation rate low reactions temperatures/irreversible deactivation of midchain radicals that can lead reduction in transient radical lifetime due to degenerative transfer process 47 to chain transfer and branching results in decrease in chain transfer to polymer and other side reactions not available
irreversible deactivation of midchain radical (applied to ATRP only)23 (note: experimental evidence shows no irreversible deactivation of midchain radical)33 midchain radical “patched” by chain transfer to CTA31 (note: experimental evidence does not show patched midchain radical)32 fast pulse prevents formation of excessive amounts of midchain radicals34
current explanation(s) observation
branching reduced in controlled radical polymerization30
Table 3. Unresolved/Ongoing Debates within Controlled Radical Polymerization That Can Be Conveniently Explained with the Linear−Exponential Distribution Model
dx.doi.org/10.1021/ma501267a | Macromolecules XXXX, XXX, XXX−XXX
(13) Ahmad, N. M.; Heatley, F.; Lovell, P. A. Chain Transfer to Polymer in Free-Radical Solution Polymerization of n-Butyl Acrylate Studied by NMR Spectroscopy. Macromolecules 1998, 31, 2822−2827. (14) Farcet, C.; Belleney, J.; Charleux, B.; Pirri, R. Structural Characterization of Nitroxide-Terminated Poly(n-butyl acrylate) Prepared in Bulk and Miniemulsion Polymerizations. Macromolecules 2002, 35, 4912−4918. (15) Junkers, T.; Barner-Kowollik, C. The Role of Mid-Chain Radicals in Acrylate Free Radical. J. Polym. Sci., Part A: Polym. Chem. 2008, 46, 7585−7605. (16) Buback, M.; Hesse, P.; Junkers, T.; Sergeeva, T.; Theis, T. PLP Labeling in ESR Spectroscopic Analysis of Secondary and Tertiary Acrylate Propagating Radicals. Macromolecules 2008, 41, 288−291. (17) Cuccato, D.; Mavroudakis, E.; Dossi, M.; Moscatelli, D. A Density Functional Theory Study of Secondary Reactions in n-Butyl Acrylate Free Radical Polymerization. Macromol. Theory Simul. 2013, 22, 127−135. (18) Heatley, F.; Lovell, P. A.; Yamashita, T. Chain Transfer to Polymer in Free-Radical Solution Polymerization of 2-Ethylhexyl Acrylate Studied by NMR Spectroscopy. Macromolecules 2001, 34, 7636−7641. (19) Thickett, S. C.; Gilbert, R. G. Midchain Transfer to Polymer in Styrene-Poly(butyl acrylate) Systems: Direct Evidence of Retardative Effects. Macromolecules 2005, 38, 9894−9896. (20) Van Herk, A. M. Historic account of the development in the understanding of the propagation kinetics of acrylate radical polymerizations. Macromol. Rapid Commun. 2009, 30, 1964−1968. (21) Van Herk, A. M. Pulsed Initiation Polymerization Applied to Acrylate Monomers: Sources of Experimental Failure. Macromol. Rapid Commun. 2001, 22, 687−689. (22) Willemse, R. X. E.; Herk, A. M. Van; Panchenko, E.; Junkers, T.; Buback, M. PLP-ESR Monitoring of Midchain Radicals in n-Butyl Acrylate Polymerization. Macromolecules 2005, 38, 5098−5103. (23) Konkolewicz, D.; Sosnowski, S.; D’hooge, D. R.; Szymanski, R.; Reyniers, M.-F.; Marin, G. B.; Matyjaszewski, K. Origin of the Difference between Branching in Acrylates Polymerization under Controlled and Free Radical Conditions: A Computational Study of Competitive Processes. Macromolecules 2011, 44, 8361−8373. (24) Peck, A. N. F.; Hutchinson, R. A. Secondary Reactions in the High-Temperature Free Radical Polymerization of Butyl Acrylate. Macromolecules 2004, 37, 5944−5951. (25) Nikitin, A. N.; Hutchinson, R. A.; Buback, M.; Hesse, P. Determination of Intramolecular Chain Transfer and Midchain Radical Propagation Rate Coefficients for Butyl Acrylate by Pulsed Laser Polymerization. Macromolecules 2007, 40, 8631−8641. (26) Arzamendi, G.; Plessis, C.; Leiza, J. R.; Asua, J. M. Effect of the Intramolecular Chain Transfer to Polymer on PLP/SEC Experiments of Alkyl Acrylates. Macromol. Theory Simul. 2003, 12, 315−324. (27) Plessis, C.; Arzamendi, G.; Leiza, R.; Schoonbrood, H. A. S.; Charmot, D.; Asua, M. Modeling of Seeded Semibatch Emulsion Polymerization of n-BA. Ind. Eng. Chem. Res. 2001, 40, 3883−3894. (28) Junkers, T.; Koo, S. P. S.; Davis, T. P.; Stenzel, M. H.; BarnerKowollik, C. Mapping Poly(butyl acrylate) Product Distributions by Mass Spectrometry in a Wide Temperature Range: Suppression of Midchain Radical Side Reactions. Macromolecules 2007, 40, 8906− 8912. (29) Koo, S. P. S.; Junkers, T.; Barner-Kowollik, C. Quantitative Product Spectrum Analysis of Poly(butyl acrylate) via Electrospray Ionization Mass Spectrometry. Macromolecules 2009, 42, 62−69. (30) Ahmad, N. M.; Charleux, B.; Farcet, C.; Ferguson, C. J.; Gaynor, S. G.; Hawkett, B. S.; Heatley, F.; Klumperman, B.; Konkolewicz, D.; Lovell, P. A.; Matyjaszewski, K.; Venkatesh, R. Chain Transfer to Polymer and Branching in Controlled Radical Polymerizations of nButyl Acrylate. Macromol. Rapid Commun. 2009, 30, 2002−2021. (31) Gaborieau, M.; Koo, S. P. S.; Castignolles, P.; Junkers, T.; Barner-Kowollik, C. Reducing the Degree of Branching in Polyacrylates via Midchain Radical Patching: A Quantitative MeltState NMR Study. Macromolecules 2010, 43, 5492−5495.
S Supporting Information *
Stochastic analysis using the classical exponential probability distribution; description of the Monte Carlo simulations for both the football example and the competitive reactions using linear−exponential probability distributions and the parameter estimation. This material is available free of charge via the Internet at http://pubs.acs.org.
*E-mail [email protected]
The authors declare no competing ﬁnancial interest.
ACKNOWLEDGMENTS Diputación Foral de Gipuzkoa, University of Basque Country (UFI 11/56), Basque Government (GVIT373-10 and Etortek Nanoiker IE11-304), and Ministerio de Economiá y Competitividad (CTQ2011-25572) are gratefully acknowledged for their ﬁnancial support.
(1) Plessis, C.; Arzamendi, G.; Leiza, J. R.; Schoonbrood, H. A. S.; Charmot, D.; Asua, J. M. Seeded Semibatch Emulsion Polymerization of n-Butyl Acrylate. Kinetics and Structural Properties. Macromolecules 2000, 33, 5041−5047. (2) Plessis, C.; Arzamendi, G.; Leiza, J. R.; Schoonbrood, H. A. S.; Charmot, D.; Asua, J. M. A Decrease in Effective Acrylate Propagation Rate Constants Caused by Intramolecular Chain Transfer. Macromolecules 2000, 33, 4−7. (3) Plessis, C.; Arzamendi, G.; Leiza, J. R.; Schoonbrood, H. A. S.; Charmot, D.; Asua, J. Kinetics and Polymer Microstructure of the Seeded Semibatch Emulsion Copolymerization of n-Butyl Acrylate and Styrene. Macromolecules 2001, 34, 5147−5157. (4) Plessis, C.; Arzamendi, G.; Alberdi, J. M.; van Herk, A. M.; Leiza, J. R.; Asua, J. M. Evidence of Branching in Poly(butyl acrylate) Produced in Pulsed-Laser Polymerization Experiments. Macromol. Rapid Commun. 2003, 24, 173−177. (5) Sato, E.; Emoto, T.; Zetterlund, P. B.; Yamada, B. Influence of Mid-Chain Radicals on Acrylate Free Radical Polymerization: Effect of Ester Alkyl Group. Macromol. Chem. Phys. 2004, 205, 1829−1839. (6) Nikitin, A. N.; Hutchinson, R. A. The Effect of Intramolecular Transfer to Polymer on Stationary Free Radical Polymerization of Alkyl Acrylates. Macromolecules 2005, 38, 1581−1590. (7) González, I.; Leiza, J. R.; Asua, J. M. Exploring the Limits of Branching and Gel Content in the Emulsion Polymerization of n-BA. Macromolecules 2006, 39, 5015−5020. (8) González, I.; Asua, J. M.; Leiza, J. R. The role of methyl methacrylate on branching and gel formation in the emulsion copolymerization of BA/MMA. Polymer 2007, 48, 2542−2547. (9) Castignolles, P.; Graf, R.; Parkinson, M.; Wilhelm, M.; Gaborieau, M. Detection and quantification of branching in polyacrylates by sizeexclusion chromatography (SEC) and melt-state 13C NMR spectroscopy. Polymer 2009, 50, 2373−2383. (10) Liang, K.; Hutchinson, R. A.; Barth, J.; Samrock, S.; Buback, M. Reduced Branching in Poly(butyl acrylate) via Solution Radical Polymerization in n-Butanol. Macromolecules 2011, 44, 5843−5845. (11) Yu-Su, S. Y.; Sun, F. C.; Sheiko, S. S.; Konkolewicz, D.; Lee, H.; Matyjaszewski, K. Molecular Imaging and Analysis of Branching Topology in Polyacrylates by Atomic Force Microscopy. Macromolecules 2011, 44, 5928−5936. (12) Agirre, A.; Santos, J. I.; Leiza, J. R. Toward Understanding the Architecture (Branching and MWD) of Crosslinked Acrylic Latexes. Macromol. Chem. Phys. 2013, 214, 589−598. J
dx.doi.org/10.1021/ma501267a | Macromolecules XXXX, XXX, XXX−XXX
(32) Agirre, A.; Santos, J. I.; Etxeberria, A.; Sauerland, V.; Leiza, J. R. Polymerization of n-butyl acrylate with high concentration of a chain transfer agent (CBr4): detailed characterization and impact on branching. Polym. Chem. 2013, 4, 2062−2079. (33) Ballard, N.; Salsamendi, M.; Santos, J. I.; Ruipérez, F.; Leiza, J. R.; Asua, J. M. Experimental Evidence Shedding Light on the Origin of the Reduction of Branching of Acrylates in ATRP. Macromolecules 2014, 47, 964−972. (34) Barner-Kowollik, C.; Günzler, F.; Junkers, T. Pushing the Limit Pulsed Laser Polymerization of n-Butyl Acrylate at 500 Hz. Macromolecules 2008, 41, 8971−8973. (35) Reyes, Y.; Asua, J. M. Revisiting chain transfer to polymer and branching in controlled radical polymerization of butyl acrylate. Macromol. Rapid Commun. 2011, 32, 63−67. (36) Hlalele, L.; Klumperman, B. Reversible Nitroxide Trapping of the Mid-Chain Radical in n-Butyl Acrylate Polymerization. Macromolecules 2011, 44, 5554−5557. (37) Reyes, Y.; Arzamendi, G.; Asua, J. M.; Leiza, J. R. Branching at High Frequency Pulsed Laser Polymerizations of Acrylate Monomers. Macromolecules 2011, 44, 3674−3679. (38) Kou, S. C.; Cherayil, B. J.; Min, W.; English, B. P.; Xie, X. S. Single-molecule Michaelis-Menten equations. J. Phys. Chem. B 2005, 109, 19068−19081. (39) Zhou, Y.; Zhuang, X. Kinetic analysis of sequential multistep reactions. J. Phys. Chem. B 2007, 111, 13600−13610. (40) Floyd, D. L.; Harrison, S. C.; van Oijen, A. M. Analysis of kinetic intermediates in single-particle dwell-time distributions. Biophys. J. 2010, 99, 360−366. (41) Daranlot, J.; Bergeat, A.; Caralp, F.; Caubet, P.; Costes, M.; Forst, W.; Loison, J.-C.; Hickson, K. M. Gas-phase kinetics of hydroxyl radical reactions with alkenes: experiment and theory. ChemPhysChem 2010, 11, 4002−4010. (42) Greenwald, E. E.; North, S. W.; Georgievskii, Y.; Klippenstein, S. J. A two transition state model for radical-molecule reactions: a case study of the addition of OH to C2H4. J. Phys. Chem. A 2005, 109, 6031−6044. (43) Greenwald, E. E.; North, S. W.; Georgievskii, Y.; Klippenstein, S. J. A two transition state model for radical-molecule reactions: applications to isomeric branching in the OH-isoprene reaction. J. Phys. Chem. A 2007, 111, 5582−5592. (44) Coelho, J. F. J.; Fonseca, a. C.; Gois, J. R.; Gonçalves, P. M. O. F.; Popov, A. V.; Gil, M. H. Scaling-up of poly(vinyl chloride) prepared by single electron transfer degenerative chain transfer mediated living radical polymerization in water media: 1) Low molecular weight. Kinetic analysis. Chem. Eng. J. 2011, 169, 399−413. (45) Percec, V.; Ramirez-Castillo, E.; Hinojosa-Falcon, L. A.; Popov, A. V. Synthesis of ultrahigh molar mass, structural defects free poly(vinyl chloride) with high syndiotacticity and glass transition temperature by single electron transfer-degenerative chain transfer living radical polymerization (SET-DTLRP). J. Polym. Sci., Part A: Polym. Chem. 2005, 43, 2185−2187. (46) Percec, V.; Popov, A. V.; Ramirez-Castillo, E.; Weichold, O. Acceleration of the single electron transfer-degenerative chain transfer mediated living radical polymerization (SET-DTLRP) of vinyl chloride in water at 25 °C. J. Polym. Sci., Part A: Polym. Chem. 2004, 42, 6364− 6374. (47) Percec, V.; Popov, A. V.; Ramirez-Castillo, E.; Coelho, J. F. J.; Hinojosa-Falcon, L. A. Non-transition metal-catalyzed living radical polymerization of vinyl chloride initiated with iodoform in water at 25 °C. J. Polym. Sci., Part A: Polym. Chem. 2004, 42, 6267−6282. (48) Coelho, J. F. J.; Fonseca, A. C.; Gonçalves, P. M. F. O.; Popov, A. V.; Gil, M. H. Particle features and morphology of poly(vinyl chloride) prepared by living radical polymerisation in aqueous media. Insight about particle formation mechanism. Polymer 2011, 52, 2998− 3010. (49) Nyström, F.; Soeriyadi, A. H.; Boyer, C.; Zetterlund, P. B.; Whittaker, M. R. End-group fidelity of copper(0)-meditated radical polymerization at high monomer conversion: an ESI-MS investigation. J. Polym. Sci., Part A: Polym. Chem. 2011, 49, 5313−5321.
(50) Percec, V.; Guliashvili, T.; Ladislaw, J. S.; Wistrand, A.; Stjerndahl, A.; Sienkowska, M. J.; Monteiro, M. J.; Sahoo, S. Ultrafast synthesis of ultrahigh molar mass polymers by metal-catalyzed living radical polymerization of acrylates, methacrylates, and vinyl chloride mediated by SET at 25° C. J. Am. Chem. Soc. 2006, 128, 14156− 14165. (51) Nguyen, N. H.; Levere, M. E.; Percec, V. SET-LRP of methyl acrylate to complete conversion with zero termination. J. Polym. Sci., Part A: Polym. Chem. 2012, 50, 860−873. (52) Jakubowski, W.; Kirci-Denizli, B.; Gil, R. R.; Matyjaszewski, K. Polystyrene with Improved Chain-End Functionality and Higher Molecular Weight by ARGET ATRP. Macromol. Chem. Phys. 2008, 209, 32−39. (53) Barner-kowollik, C.; Buback, M.; Charleux, B.; Coote, M. L.; Drache, M.; Fukuda, T.; Goto, A.; Klumperman, B.; Lowe, A. B.; Mcleary, J. B.; Moad, G.; Monteiro, M. J.; Sanderson, R. D.; Tonge, M. P.; Vana, P.; Marie, P. Mechanism and Kinetics of DithiobenzoateMediated RAFT Polymerization. I. The Current Situation. J. Polym. Sci., Part A: Polym. Chem. 2006, 44, 5809−5831. (54) Moad, G. Mechanism and Kinetics of Dithiobenzoate-Mediated RAFT Polymerization - Status of the Dilemma. Macromol. Chem. Phys. 2014, 215, 9−26. (55) Geelen, P.; Klumperman, B. Intermediate Radical Termination in Reversible Addition-Fragmentation Chain Transfer-Mediated Polymerization: Identification of Termination Products. Macromolecules 2007, 40, 3914−3920. (56) Calitz, F. M.; McLeary, J. B.; McKenzie, J. M.; Tonge, M. P.; Klumperman, B.; Sanderson, R. D. Evidence for Termination of Intermediate Radical Species in RAFT-Mediated Polymerization. Macromolecules 2003, 36, 9687−9690. (57) Konkolewicz, D.; Hawkett, B. S.; Gray-Weale, A.; Perrier, S. RAFT Polymerization Kinetics: Combination of Apparently Conflicting Models. Macromolecules 2008, 41, 6400−6412. (58) Feldermann, A.; Coote, M. L.; Stenzel, M. H.; Davis, T. P.; Barner-Kowollik, C. Consistent experimental and theoretical evidence for long-lived intermediate radicals in living free radical polymerization. J. Am. Chem. Soc. 2004, 126, 15915−15923. (59) Soeriyadi, A. H.; Boyer, C.; Nyström, F.; Zetterlund, P. B.; Whittaker, M. R. High-order multiblock copolymers via iterative Cu(0)-mediated radical polymerizations (SET-LRP): toward biological precision. J. Am. Chem. Soc. 2011, 133, 11128−11131. (60) Wang, Y.; Soerensen, N.; Zhong, M.; Schroeder, H.; Buback, M.; Matyjaszewski, K. Improving the “Livingness” of ATRP by Reducing Cu Catalyst Concentration. Macromolecules 2013, 46, 683− 691. (61) Zhong, M.; Matyjaszewski, K. How Fast Can a CRP Be Conducted with Preserved Chain End Functionality? Macromolecules 2011, 44, 2668−2677. (62) Konkolewicz, D.; Wang, Y.; Zhong, M.; Krys, P.; Isse, A. A.; Gennaro, A.; Matyjaszewski, K. Reversible-Deactivation Radical Polymerization in the Presence of Metallic Copper. A Critical Assessment of the SARA ATRP and SET-LRP Mechanisms. Macromolecules 2013, 46, 8749−8772.
dx.doi.org/10.1021/ma501267a | Macromolecules XXXX, XXX, XXX−XXX